1. Chapter 1 Introduction to PiezoelectricityThis chapter provides a basic introduction to piezoelectricity. It begins with a dis-cussion of background and applications of piezoelectric materials. We then presentthe linear theory of piezoelectricity, functionally graded piezoelectric materi-als(FGPM), and fundamental knowledge of fibrous piezoelectric composites(FPC).1.1 BackgroundPiezoelectric material is such that when it is subjected to a mechanical load, it gen-erates an electric charge (see Fig. 1.1(a)). This effect is usually called the “piezo-electric effect”. Conversely, when piezoelectric material is stressed electrically by avoltage, its dimensions change (see Fig. 1.1(b)). This phenomenon is known as the“inverse piezoelectric effect”. The direct piezoelectric effect was first discovered bythe brothers Pierre Curie and Jacques Curie more than a century ago . Theyfound out that when a mechanical stress was applied to crystals such as tourmaline,topaz, quartz, Rochelle salt and cane sugar, electrical charges appeared, and thisvoltage was proportional to the stress.Fig. 1.1 Electroelastic coupling in piezoelectricity.(a) Piezoelectric effect: voltage inducedby force. (b) Inverse piezoelectric effect: strain induced by voltage.The Curies did not, however, predict that crystals exhibiting the direct piezo-electric effect (electricity from applied stress) would also exhibit the inverse piezo-electric effect (strain in response to applied electric field). One year later that prop-erty was theoretically predicted on the basis of thermodynamic consideration byLippmann , who proposed that converse effects must exist for piezoelectricity,pyroelectricity (see Fig. 1.2), etc. Subsequently, the inverse piezoelectric effect wasconfirmed experimentally by Curies , who proceeded to obtain quantitative proofof the complete reversibility of electromechanical deformations in piezoelectriccrystals. These events above can be viewed as the beginning of the history of piezo-Q.-H. Qin, Advanced Mechanics of Piezoelectricity© Higher Education Press, Beijing and Springer-Verlag Berlin Heidelberg 2013
2. 2 Chapter 1 Introduction to Piezoelectricityelectricity. Based on them, Woldemar Voigt  developed the first complete andrigorous formulation of piezoelectricity in 1890. Since then several books on thephenomenon and theory of piezoelectricity have been published. Among them arethe books by Cady , Tiersten , Parton and Kudryavtsev , Ikeda , Ro-gacheva , Qin [10,11], and Qin and Yang . The first  treated the physicalproperties of piezoelectric crystals as well as their practical applications, the second dealt with the linear equations of vibrations in piezoelectric materials, and thethird and fourth [7,8] gave a more detailed description of the physical properties ofpiezoelectricity. Rogacheva  presented general theories of piezoelectric shells.Qin [10,11] discussed Green’s functions and fracture mechanics of piezoelectricmaterials. Micromechanics of piezoelectricity were discussed in .Fig. 1.2 Illustration of pyroelectricity.In general, the piezoelectric effect occurs only in nonconductive materials. Pie-zoelectric materials can be divided into two main groups: crystals and ceramics.The best known piezoelectric material in the crystal group is quartz (SiO2), thetrigonal crystallized silica which is known as one of the most common crystals onthe earth’s surface. In the ceramics group, a typical piezoelectric material is bariumtitanate (BaTiO3), an oxide of barium and titanium.It should be mentioned that an asymmetric arrangement of positive and negativeions imparts permanent electric dipole behavior to crystals. In order to “activate”the piezo properties of ceramics, a poling treatment is required. In that treatment thepiezo ceramic material is first heated and an intense electric field (> 2 000 V/mm) isapplied to it in the poling direction, forcing the ions to realign along this “poling”axis. When the ceramic cools and the field is removed, the ions “remember” thispoling and the material now has a remanent polarization (which can be degraded byexceeding the mechanical, thermal and electrical limits of the material). Subse-quently, when a voltage is applied to the poled piezoelectric material, the ions in theunit cells are shifted and, additionally, the domains change their degree of align-ment. The result is a corresponding change of the dimensions (expansion, contrac-tion) of the lead zirconate titanate (PZT) material. In the poling treatment, the Curietemperature is the critical temperature at which the crystal structure changes from anonsymmetrical (piezoelectric) to a symmetrical (non-piezoelectric) form. Particu-larly, when the temperature is above the Curie temperature, each perovskite crystal
3. 1.1 Background 3(perovskite is a calcium titanium oxide mineral species composed of calciumtitanate, with the chemical formula CaTiO3) in the fired ceramic element exhibits asimple cubic symmetry with no dipole moment (Fig. 1.3(a)). At temperatures belowthe Curie point, however, each crystal has tetragonal or rhombohedral symmetryand a dipole moment (Fig. 1.3(b)).Fig. 1.3 Crystal structures with the Curie temperature.(a) Temperature above Curie temperature:symmetric. (b) Temperature below Curie temperature: non-symmetric.Although piezoelectricity was discovered in 1880 it remained a mere curiosityuntil the 1940s. The property of certain crystals to exhibit electrical charges undermechanical loading was of no practical use until very high input impedance ampli-fiers enabled engineers to amplify their signals. In 1951, several Japanese compa-nies and universities formed a “competitively cooperative” association, establishedas the Barium Titanate Application Research Committee. This association set anorganizational precedent not only for successfully surmounting technical challengesand manufacturing hurdles, but also for defining new market areas. Persistent ef-forts in materials research created new piezoceramic families which were competi-tive with Vernitron’s PZT. With these materials available, Japanese manufacturersquickly developed several types of piezoelectric signal filters, which addressedneeds arising from television, radio, and communications equipment markets; andpiezoelectric igniters for natural gas/butane appliances. As time progressed, themarkets for these products continued to grow, and other similarly lucrative oneswere found. Most notable were audio buzzers (smoke alarms), air ultrasonic trans-ducers (television remote controls and intrusion alarms) and devices employingsurface acoustic wave effects to achieve high frequency signal filtering.The commercial success of the Japanese efforts attracted the attention of indus-try in many other countries and spurred new efforts to develop successful piezo-electric products. There has been a large increase in relevant publications in China,India, Russia and the USA. Since the piezoelectric effect provides the ability to usethese materials as both sensors and actuators, it has found relevant applications re-quiring accurate measurement and recording of dynamic changes in mechanicalvariables such as pressure, force and acceleration. The list of applications continues
4. 4 Chapter 1 Introduction to Piezoelectricityto grow and now includes  (a) aerospace: model testing, wind tunnel and shocktube instrumentation, landing gear hydraulics, rocketry, structures, ejection systemsand cutting force research; (b) ballistics: combustion, explosion, detonation andsound pressure distribution; (c) biomechanics: multi-component force measurementfor orthopedic gait and posturography, sports, ergonomics, neurology, cardiologyand rehabilitation; (d) engine testing: combustion, gas exchange and injection, in-dicator diagrams and dynamic stressing; (e) engineering: materials evaluation, con-trol systems, reactors, building structures, ship structures, auto chassis structuraltesting, shock and vibration isolation and dynamic response testing; (f) indus-trial/manufacturing: machining systems, metal cutting, press and crimp force,automation of force-based assembly operations and machine health monitoring; and(g) OEMs (original equipment manufacturer): transportation systems, plastic mold-ing, rockets, machine tools, compressors, engines, flexible structures, oil/gas drill-ing and shock/vibration testers.Judging by the increase in worldwide activity focused on using a large numberof very precise piezoelectric sensors and actuators for active control in communica-tions, navigation and packaging systems, and from the successes encountered in thelast sixty years, it is expected that piezoelectricity will enjoy a continuing role inboth fundamental and technical applications in the future.In this chapter, the linearized piezoelectric formulations described in [10,11,14],the concept of FGPM and fiber piezocomposites, which will be needed in laterchapters, are briefly summarized. The basic equations of linear electroelasticity arefirst reviewed, followed by a brief discussion of FGPM and FPC, which have im-portant applications in practical engineering. Then some issues in interface andfracture mechanics in piezoelectricity are outlined.1.2 Linear theory of piezoelectricity1.2.1 Basic equations in rectangular coordinate systemThis section recalls briefly the three-dimensional formulation of linear piezoelec-tricity that appeared in [11,14]. Here, a three-dimensional Cartesian coordinate sys-tem is adopted where the position vector is denoted by x (or xi). In this book, bothconventional indicial notation xi and traditional Cartesian notation (x, y, z) are util-ized. In the case of indicial notation we invoke the summation convention over re-peated Latin indices, which can be of two types with different ranges: i, j, k=1,2,3for lower-case letters and M, N=1,2,3,4 for upper-case letters. Moreover, vectors,tensors and their matrix representations are denoted by bold-face letters. Thethree-dimensional constitutive equations for linear piezoelectricity can be derived
5. 1.2 Linear theory of piezoelectricity 5by considering an electric enthalpy function H defined as 1 1( , )2 2Eijkl ij kl ij i j kij ij kH c E E eE E (1.1)where the strain tensor and the electric field vector are related tothe displacement u and the electric potential by( )ij ( )iEE, ,1( ),2ij i j j i i iu u E , (1.2)in which a comma followed by arguments denotes partial differentiation with re-spect to the arguments, Eijklc , are the elastic, piezoelectric, and dielec-tric constants, respectively. The superscript E inandkij ijeEijklc indicates that the elastic con-stants are measured at a constant electric field. The superscript in indicatesthat the dielectric constants are measured at a constant strain. To simplify subse-quent writing, we shall omit the superscripts E and in the remaining part of thisbook. The material constants in Eq. (1.1) can be reduced by the following consid-eration. According to the definition (1.2) we may write ij= ji. It follows thatij(1.3)ijkm ijmkc cFurther, from we haveij ji(1.4),ijkm jikm kij kjic c e eIn view of these properties, it is useful to introduce the so-called two-index no-tation or compressed matrix notation . Two-index notation consists of replacingij or km by p or q, i.e. cijkm=cpq, eikm=eiq, ij= p when i=j, and 2 ij= p when i j,where i, j, k, m take the values 1-3, and p, q assume the values 1-6 according to thefollowing replacements 11 1, 22 2, 33 3, 23 or 32 4, 13 or 31 5, 12 or21 6.Constitutive relations are obtained from the electric enthalpy function (1.1) as( , ),( , )ij ijkl kl kij kiji ikl kliHc e EHD eEEEik kEkE(1.5)where is the stress tensor and Di the electric displacement vector. Making useof two-index notation mentioned above, Eqs. (1.5) are reduced toij(1.6),p pq q kp k i iq q ikc E D e
6. 6 Chapter 1 Introduction to Piezoelectricityin which(1.7)(when )2 (when )ijpiji ji jIn addition to the constitutive relation (1.5) above, three other forms of constitu-tive representation are commonly used in the linear theory of piezoelectricity todescribe the coupled interaction between elastic and electric variables . Eachtype has its own different set of independent variables and corresponds to a differ-ent electric enthalpy function, as listed in Table 1.1. It should be pointed out that analternative derivation of formulae is merely a transformation from one type of rela-tion to another. Some relationships between various constants occurring in the fourtypes are as follows:(1.8)1 T 11 1 T1 1( ) , , , ( ) ( ) ,( ) , ( ) , ( ) ,( ) , ( )E E E e D ED E E E Ec f e c d d c d f c d dg d c c c d d c h c d1 T1Table 1.1 Four types of fundamental electroelastic relations.Independent variables Constitutive relations Electric enthalpy functional, ETEc e ED e E0H =12cE 2–12E2–e E, DTDc h DE h D1H = +ED0H,ETEf d ED d E2H = –0H, DTDf g DE g D3H = + ED –0HHaving defined constitutive relations, the related divergence equations andboundary conditions can be derived by considering the generalized variational prin-ciple :[ ( , ) ]d d d 0t qi i i i sH f u Q t u s q sE (1.9)where is the variational symbol, fi the body force vector, Q the electric chargedensity, and is the solution domain. t and q are the boundaries on which thesurface traction and surface charge are prescribed, respectively. andit sq are theprescribed surface traction and surface charge, respectively.
7. 1.2 Linear theory of piezoelectricity 7The variational equation (1.9) provides the following results:(in ) (1.10), ,0, 0ij j i i if D Q(on ), (on )ij j i t i i s qn t D n q (1.11)and the constitutive equations (1.5), where ni is the unit outward normal vector to .Equations (1.10) are the elastic equilibrium equations and Gauss’ law of electro-statics, respectively, Eqs. (1.11) are boundary conditions and Eqs. (1.5) the constitu-tive equations.The boundary value problems defined by Eqs. (1.2), (1.5), (1.10), and (1.11)should be completed by the following essential boundary conditions:(on ), (on )i i uu u (1.12)where andiu are prescribed displacements and electrical potential, and u andare the parts of ( u t q ) on which the displacement andelectric potential are prescribed, respectively.Substitution of Eq. (1.2) into Eq. (1.6), and later into Eq. (1.10), results in11 1,11 11 12 2,12 13 44 3,13 11 12 1,221 1( ) ( ) ( )2 2c u c c u c c u c c u44 1,33 31 15 ,13 1( )c u e e f 0 (1.13)11 2,22 11 12 1,12 13 44 3,23 11 12 2,111 1( ) ( ) ( )2 2c u c c u c c u c c u(1.14)44 2,33 31 15 ,23 2( )c u e e f 044 3,11 44 13 1,31 2,32 44 3,22 33 3,33( )( )c u c c u u c u c u( ) 0e e f15 ,11 ,22 33 ,33 3 (1.15)15 3,11 3,22 15 31 1,31 2,32 33 3,33( ) ( )( )e u u e e u u e u( ) 0Q (1.16)11 ,11 ,22 33 ,33for transversely isotropic materials (class C6v=6mm) with x3 as the poling directionand the x1-x2 plane as the isotropic plane.1.2.2 Boundary conditionsIn electroelasticity theory, mechanical boundary conditions are formulated just as inclassical elasticity theory. The electric boundary conditions are, however, still de-bated. The first attempt to define the electric boundary conditions over crack faceswas by Parton . He assumed that although the magnitude of the normal electri-
8. 8 Chapter 1 Introduction to Piezoelectricitycal displacement component at the crack face is very small, the electrical displace-ment is continuous across the crack faces. He used the following electric boundaryconditions:(1.17), nD Dn)Later, Hao and Shen  improved on the above assumption by considering theelectric permeability of air in the crack gap. In addition to Eq. (1.17), they presentedan equation for the boundary condition at crack faces:(1.18), ( ) (n n n n n aD D D u uwhere a is the permittivity of air. However, Eq. (1.18) has for a long time remaineddisregarded due to its complex mathematical treatment.As pointed out by Suo et al. , the above assumption is not physically realis-tic as there will clearly be a potential drop across the lower capacitance crack. Thisis particularly true for those piezoelectric ceramics with permittivity 103timeshigher than the environment (e.g. air or vacuum). For this reason, Deeg  pro-posed another set of electric boundary conditions over crack faces:(1.19)0n nD DEquation (1.19) are derived from the constitutive equation Dn= aEn. This isequivalent to having crack surfaces free of surface charge as the electrical boundarycondition, and thus the electric displacement vanishes in the environment. We adoptEq. (1.19) in most of the subsequent chapters because of its much simpler mathe-matical treatment and the fact that the dielectric constants of a piezoelectric materialare much larger than those of the environment (generally between 1 000 and 3 500times greater).1.3 Functionally graded piezoelectric materialsFunctionally graded materials (FGMs) are composite materials formed of two ormore constituent phases with a continuously variable composition. This feature caneliminate the stress discontinuity that is often encountered in laminated compositesand thus can avoid delamination-related problems. Traditionally, homogeneouslaminas with different properties are bonded together to form laminated compositestructures for engineering applications. The discontinuity of material propertiesacross adjoining layers in a laminated composite can, however, result in crack ini-tiation or delamination at the interfaces. To mitigate those disadvantages of lami-nated composite structures, a new class of piezoelectric materials called FGPMs hasrecently been developed. The FGPM is a kind of piezoelectric material intentionallydesigned to possess desirable properties for specific applications, and featuring ma-
9. 1.3 Functionally graded piezoelectric materials 9terial composition and properties varying continuously in desired direction(s).Smart structures or elements made of FGPM are thus superior to conventional sen-sors, and actuators are often made of uni-morph, bi-morph and multimorph materi-als. This is because, for piezoelectric laminates with layered materials having ho-mogeneous properties, large bending displacements, high stress concentrations,creep at high temperature and failure from interfacial bonding frequently occur atthe layer interfaces under mechanical or electric loading. These effects can lead toreduced reliability and lifespan.1.3.1 Types of gradationThe mechanical, electrical, magnetic, and thermal properties of FGMs are usuallyassumed to have the same functions of certain space coordinates. Three com-monly-used graded forms are.(1) Exponential material gradation.All the material constants including elastic constants, piezoelectric parameters,dielectric constants, thermal expansion coefficients, and material density follow theexponential law:0 xij ijM M e (1.20)where Mij represents material constants such as cij, or fij, 0ijM are the correspondingvalues at the plane x=0, and denotes a material graded parameter.(2) Quadratic material gradation.All material constants are assumed to have the same power-law dependence onthe coordinate x:0(1 )nij ijM M x (1.21)where n is the inhomogeneous constant determined empirically.(3) Trigonometric material gradation.For some special applications, the material constants of FGMs may follow atrigonometric law as (1.22)01 2 2( cos sin )nij ijM M a X a X2where a1, a2, and n are four material constants.1.3.2 Basic equations for two-dimensional FGPMsThe field equations of electroelasticity reduce to two-dimensional form in two spe-cial cases which are of some interest.
10. 10 Chapter 1 Introduction to Piezoelectricity(1) Plane strain.Consider a transversely isotropic FGPM. In this case, according to Eq. (1.6), thex-y plane is the isotropic plane, and one can employ either the x-z or y-z plane forthe study of plane electromechanical phenomena. Choosing the former, the planestrain conditions require that0 (1.23)yy zy xy yEBy substitution of Eq. (1.23) into Eq. (1.6), we have11 13 3113 33 3355 1515 1131 33 330 00 00 0 00 0 00 0x xz zxz xzx xz zc c ec c ec eeD Ee eD E(1.24)or inversely11 13 3113 33 3355 1515 1131 33 330 00 00 0 00 0 00 0x xz zxz xzx xz za a ba a ba bbE Db bE D(1.25)where aij, bij and ij are the reduced material constants. They are related to the elas-tic compliance tensor fij, the piezoelectric tensor gij, and the dielectric impermeabil-ity tensor ij by the following relations :2212 13 131211 11 13 13 33 33 55 55 15 1511 11 11231 12 31 13 3131 31 33 33 11 11 33 3311 11 11, , , , ,, , ,f f ffa f a f a f a f b gf f fg f g f gb g b gf f f1.26with fij, gij and ij being defined in Table 1.1. In the constitutive equations (1.39) and(1.40), –Ei is used instead of Ei because it will allow the construction of a symmetricgeneralized linear response matrix which will prove to be advantageous. When theconstitutive equation (1.24) is substituted into Eq. (1.10) we obtain11 1,1 13 3,3 31 ,3 55 3,1 1,3 15 ,1 1,1 ,3[ ]c u c u e c u u e f 0 (1.27)55 3,1 1,3 15 ,1 13 1,1 33 3,3 33 ,3 3,1 ,3[ ]c u u e c u c u e f 0 (1.28)
11. 1.4 Fibrous piezoelectric composites 1115 3,1 1,3 11 ,1 31 1,1 33 3,3 33 ,3,1 ,3[ ]e u u e u e u Q 0U(1.29)in which the material constants are functions of coor-dinates. When the Airy stress function approach is used to solve this equation [, , , , , andij ij ij ij ij ijc e a b21],the solution can be divided into two major parts: a homogeneous solution part and aparticular solution part. For the homogeneous solution part, the required straincompatibility equation and the Airy function U are, respectively, expressed by(1.30)1,33 3,11 13,13 0(1.31),33 ,11 ,13, ,x z xzU UFor most applications of FGPMs, the material properties are designed to vary con-tinuously in one direction only, say, the z-direction. Substituting Eqs. (1.2), (1.24),(1.25), and (1.31) into Eqs. (1.30) and (1.29), we have 31 ,33 33 ,11 15 ,113 33 ,3 11 ,11,3 ,3 ,3b U b U b U (1.32)11 ,33 13 ,11 55 ,113 13 ,1133 33 ,1111,33 ,3a U a U a U a U a U13 ,3 33 ,113 15 ,11,33 ,3b b b (1.33)(2) Anti-plane deformation.In this case only the out-of-plane elastic displacement u3 and the in-plane elec-tric fields are non-zero, i.e.,(1.34)0, ( , ),( , ), ( , ), 0x x y y zu v w w x yE E x y E E x y EThus the constitutive equation (1.6) is simplified to55 1555 1515 1115 110 00 00 00 0xz xzyz yzx xy yc ec eD eD EeE(1.35)The governing equations (1.10) become44 3,1 15 ,1 44 3,2 15 ,2 3,1 ,215 3,1 11 ,1 15 3,2 11 ,2,1 ,200c u e c u e fe u e u Q(1.36)1.4 Fibrous piezoelectric compositesDue to the coupling effect between mechanical and electrical fields, piezoelectric
12. 12 Chapter 1 Introduction to Piezoelectricitymaterials have been widely used in smart structures and other applications such aselectromechanical sensors, ultrasonic transducers, hydrophones, micropositioningdevices, buzzers, accelerometers, and structural actuators . However, whenserving as sensors and actuators, single-phase piezoelectric ceramic materials areoften unable to meet the increased demands from modern industry for high me-chanical performance and special structural functions, because of their intrinsicbrittleness and the existence of microcracks and defects in most piezoelectric ce-ramic materials. To overcome these drawbacks, piezoelectric material is usuallyembedded in non-piezoelectric materials in the form of fiber-matrix composites. A composite configuration for structural actuation with significant advantagesover conventional piezoelectric actuators has been conceived, and the recent deve-lopment of piezoelectric ceramic fibers <100 m in diameter has enabled this con-cept to be realized. Nelson  has predicted that FPCs will find uses in contourcontrol, non-destructive testing, vibration suppression, and noise control. The pos-sibility of computer control using closed loop systems has led to FPC emerging asfavored candidates for “smart” materials and structures. The first FPC were devel-oped in the Active Materials and Structures Laboratory at the Massachusetts Insti-tute of Technology and patented in 2000 . Typically, an FPC comprises amonolayer of uniaxially aligned piezoelectric fibers embedded in a polymer matrixbetween two interdigitated surface electrodes through which the driving voltage issupplied. Since their initial development, significant advances have been made inmany areas including fiber manufacture, matrix materials and design, electrodedesign, manufacturing techniques, and composite modeling.At this time, various FPCs are used in practical engineering including:(1) 1-3 piezo fiber composites.The 1-3 piezoelectric composite is the classification given in Newnham’s con-nectivity theory  for the identification of composites containing piezoelectricceramic rods in a polymer matrix. In Newnham’s connectivity theory there are tenimportant connectivity patterns in diphasic solids: 0-0, 1-0, 2-0, 3-0, 1-1, 2-1, 3-1,2-2, 3-2, and 3-3. A 3-1 (or 1-3) connectivity pattern, for example, has one phaseself-connected in three-dimensional layers, the other self-connected inone-dimensional chains. The 1-3 piezo fiber composites are produced with the aimof obtaining a combination of piezoelectric and mechanical properties which areuseful in electromechanically transducing applications. In the 1-3 connectivity, par-allel fibers are embedded in a matrix in the longitudinal (z) direction. Work on pie-zoelectric materials in transducers highlights the fact that piezoelectric compositeshave more desired properties than single phase piezoelectric materials. For example,a composite with PZT volume fraction of 40% can have a value of d33, almost thesame as the PZT ceramic itself.Various fabrication processes exist for different configurations and connectivi-ties of FPCs. In general, the fabrication processes include poling of the PZT fi-
13. 1.4 Fibrous piezoelectric composites 13bers/rods; the fibers are arranged in a mold, infiltrated with epoxy, cured, and dicedto produce cube-shaped blocks; the composite can be poled at the very last stage orthe fibers can be prepoled before embedding in the matrix. A typical method of fab-ricating composites presented in  is casting the polymer around the aligned PZTrods, the “lost wax” method, the “dice-and-fill” technique and a lamination process.PZT fibers may be produced by sol-gel processing, the relic process, or the viscoussuspension spinning process . Several processes using different organic solu-tions were prepared in terms of the stiffness of the fibers and compaction . Itwas found that when a certain amount of specified solutions was added, the flexi-bility and compaction of the resulting fibers were optimized.The material parameters for composites, such as compliance, stiffness, permi-ttivity and piezoelectric constants, are obviously dependent on the arrangement ofthe matrix and fibers in the composite. Calculation of effective composite parame-ters as a function of volume fraction is based on the rules of mixture . The cal-culation is based on the following assumptions: (a) Composite strain in the longitu-dinal direction (z) is equal to the fiber strain and also to the matrix in the same di-rection, and longitudinal composite stress is the weighted sum of the matrix stressand the fiber stress. (b) Lateral composite stress is equal to lateral fiber stress andalso to the matrix stress, and lateral composite strain is the weighted sum of thecorresponding matrix and fiber strains. (c) Longitudinal composite electric field isthe same as that of matrix and also that of fiber. There is no lateral composite elec-tric field. (d) Longitudinal composite electric displacement is the weighted sum ofmatrix and fiber electric displacement. It should be mentioned that most piezoelec-tric 1-3 fiber composite micromechanics models were initially developed for ultra-sonic transducer applications, but their methods can be applied to applications ofpiezoelectric fiber composites in other smart structures. A review of the 1-3 piezo-electric composite in high-frequency (0.5 MHz) applications was given in .(2) FPC with interdigitated electrodes (IDE).The 1-3 piezo composites have already demonstrated substantial advantagesover monolithic piezoelectric ceramics, but, as indicated in , one major draw-back remains from the previous work in 1-3 piezo composites low actuation per-formance. The high dielectric mismatch between fiber and matrix (approximatelythree orders of magnitude in size) seriously reduces the electric field available to thefiber material for actuation. Furthermore, high field concentrations in the poly-mer-based matrix often cause dielectric breakdown prior to poling. These problemscan be addressed by introducing IDE technology into FPCs . In 1993, Hagoodet al.  developed something similar to a circuit layer with electrodes, called IDE,and placed them on the top and bottom surfaces of the piezoceramic layer. Thisallowed the electric field to be applied in the transverse direction of a piezoceramic,thus maximizing the transverse actuation. Later Bent and Hagood  introducedIDE to FPCs. As shown in Fig. 1.4 there are three main constituents of an FPC-IDE:
14. 14 Chapter 1 Introduction to Piezoelectricitypiezoelectric fibers, IDE and a polymer matrix. The fibers are typically circular incross section and made by an extrusion process, but can also be fabricated usingmolding techniques or by slicing monolithic piezoelectric sheets to obtain fibers ofrectangular cross section. The metallic electrodes are normally made using photo-lithography. The polymeric matrix material is perhaps the constituent with the wid-est range of acceptable materials. Ideally, the matrix will have outstanding me-chanical, and dielectric properties and will bond to the fibers in a consistent manner.Fig. 1.4 FPC with IDE.In the FPC-IDE shown in Fig. 1.4, fibers are aligned in plane, with orientationalong the z-axis, while matrix material provides the load transfer and distributionalong the fibers. The electrode patterns have fingers of alternating polarity, and ex-act mirror images on the top and bottom faces. Poling is predominantly along thez-axis direction. Application of an electric field produces primary actuation alongthe fibers and transverse actuation perpendicular to the fibers.To model and investigate the improvement in the effective properties of FPCwith IDE, Bent and Hagood  used an analytical model based on the uniformfields model (UFM) and a finite element model, both of which were formulated fora representative volume element (RVE). The UFM is a generalization of thewell-known “rule of mixture” which uses parallel and series (Voight and Reuss)additions to model the effective properties of two-phase materials. The FPC consistsof PZT fibers aligned within a graphite/epoxy lamina and is sandwiched betweenthe IDE. As the name implies, the UFM assumes that the fields within the structureare uniform. The rest of the formulation is based on rules analogous to the rule ofmixture for combining two different phases/materials in various configurations.This led to the development of combination models for more complex arrangementsof the two phases. The UFM method, in fact, violates compatibility and equilibriumat some material interfaces. However, the large material mismatches make thismethod particularly well suited to modeling these types of composites .
15. 1.4 Fibrous piezoelectric composites 15(3) Hollow tube FPC.Although FPC-IDE based on solid cross-section piezoelectric fibers are veryuseful for both longitudinal and transverse activation, they require high voltagesand are constrained to nonconductive matrix materials. Particularly, they require theelectric field to pass through the composite matrix. Due to the placement of theelectrode on the matrix surface, electric field losses are significant, requiring highvoltages for actuation. Moreover, the FPC-IDE limit the matrix to electrically non-conductive materials, which is particularly a problem in large structure and air ve-hicle applications where metals and carbon fiber composites are almost exclusivelyutilized in construction. To overcome these drawbacks, a new type of FPC has beenfabricated using extruded hollow cross-section fibers . Use of FPCs with hollowcross-section piezoelectric fibers can lower operating voltages and broaden thechoice of possible matrix materials. In the hollow tube FPC, hollow fibers are indi-vidually electroded on both the inside and outside surfaces . They are activatedby an electric field applied directly across the walls of the fiber, generating longitu-dinal strain due to piezoelectric d31 mode. Even though the longitudinal strain isdecreased by approximately half by using d31 versus the d33 mode used in solid fiberFPCs, the required voltage can be decreased by a factor of 10 or more since theelectric field is applied only across the wall of the fiber instead of through the ma-trix, thereby eliminating field losses .Several existing processes, based on molding or extrusion techniques, areavailable for fabricating hollow piezoelectric fibers . Since the fibers have smalldiameters, on the order of 0.9 mm, a new manufacturing technique has been im-plemented called microfabrication by coextrusion (MFCX) . MFCX is capableof inexpensively producing long ceramic forms (>100 mm long) with complexcross-section and small features. Manufacturing of fibers with MFCX consists ofthree major steps, formation of feed rod, extrusion, and burnout/sintering . Asdescribed in , the feed rod formation process has two main steps. The first is tomix piezoelectric powder with thermoplastic polymers and to separately mix thesame polymers with carbon black powder so that the two mixes have nearly thesame viscosity. The piezoelectric mix is then formed into a round, thick-walled tube,while part of the carbon black mix is formed into a round cylinder with diameterexactly the same as the inside of the piezoelectric tube. The remainder of the carbonblack mix is formed into a square cross-section block with the same dimension asthe inlet to the extrusion die, while a circular hole is bored into the center of thesquare, with exactly the same diameter as the outside of the piezo tube. These threecomponents are then assembled, with the carbon black cylinder inside the hollowpiezo tube, which in turn is placed inside the square block. The extrusion processbegins when the assembled feed rod is heated and inserted into the extrusion die,which turns to reducing the cross-section of the feeder rod by a factor of 25 or 40,depending on the desired final tube dimensions. The resulting “green” fibers are
16. 16 Chapter 1 Introduction to Piezoelectricitythen heated to and held at 1 300 for 48 hours during the burnout and sinteringstep. This causes the carbon to be burned off from the exterior and interior of thetube and causes the thermoplastics to be removed from the piezoceramic material,which produces a stronger, denser ceramic and is accompanied typically by a 30%reduction in the cross-section of the finished hollow tube.To assess the strain response of a piezo tube FPC under an electric field, Zhanget al.  presented a simple model detailed as follows: For a tubular structure, thecylindrical polar coordinate system (r, , z) as shown in Fig. 1.5 is used. The prob-lem is assumed to be axi-symmetric and all fields are independent of polar angleand the displacement u =0. To simplify the analysis it is further assumed that thecoupling terms containing both r and z in the displacements field can be neglectedand ur = ur(r), uz = uz(z). Under these assumptions, the non-zero strain componentsare(1.37), , / ,r r r r z zu u r ,zuFig. 1.5 Schematic drawing of a piezoelectric tube.Making use of the constitutive equation (1.6), we have11 12 12 3312 11 12 3112 12 11 31,,r r zr zrrz r zc c c e Ec c c e Ec c c e Er(1.38)where Er is the applied electric field on the tube wall along the r direction. It is ob-vious that the electric field is not a constant inside the tube wall, and with a totalvoltage V applied on the tube, . In writing Eq.(1.38), Zhang et al. [0 0 0 0/[ ln( / )] ( )rE V r R r r r R36] also made the assumption that the tube is elastically iso-tropic to simplify the analysis. Making use of the equilibrium equation (1.10) andEqs. (1.38), we can derive the basic elastic equations for this problem
17. References 171131 ,,,(1 )(1 2 )1 1, cons1r r z zrraru e E ur rtant (1.39)where a11 is defined in Eq. (1.26), and is the Poisson’s ratio. The solutions to Eq.(1.39) are then(1.25)31 110 0(1 )(1 2 ),ln( / ) 1r ze V abu ar u czr R r(1.40)in which a, b, and c are the integration constants which can be determined from theboundary conditions: 31 ,z md E0 0 )ln( /R rwhere Em is the average electric field in thetube and at r =R0 and r0 there is no external stresson the tube wall, which implies r=0 at these two boundaries. Substituting Eq. (1.40)into Eq. (1.38) and using the boundary conditions, we obtain0 02 /[( )];mE V R r33 31 33 310 0 31(1 2 ), ,2(1 ) 2(1 )m md d d da E b R r E c d Em (1.41)All the strain components for the tube can be obtained from Eqs. (1.40) and (1.41).Making use of the solution, Zhang et al.  analyzed a typical hollow tube FPCand found that the effective piezoelectric constant in the radial direction of a tubecould be changed from positive to negative by adjusting the ratio R0 /r0 for piezo-electric materials. Therefore, it is possible to make a piezoelectric transducer withall the effective piezoelectric tensile constants having the same sign.References Curie J, Curie P: Development par compression de l’eletricite polaire dans les cristauxhemiedres a faces inclines. Bulletin no. 4 de la Societe Mineralogique de France 3,90(1880) and Comptes Rendus Acad. Sci. Paris 91, 294 (1880). Lippmann HG: Sur le principe de la conversation de l’eletricite ou second principe dela theorie des phenomenes electriques. Comptes Rendus Acad. Sci. Paris 92, 1049(1881). Curie J, Curie P: Contractions et dilations productes par des tensions electriques dansles cristaux hemiedres a faces inclines. Comptes Rendus Acad. Sci. Paris 93, 1137(1884). Voigt W: General theory of the piezo and pyroelectric properties of crystals. Abh. Gott.36, 1 (1890). Cady WG: Piezoelectricity, Vol. 1 & 2. Dover Publishers, New York (1964). Tiersten HF: Linear Piezoelectric Plate Vibrations. Plenum Press, New York (1969). Parton VZ, Kudryavtsev BA: Electromagnetoelasticity, Piezoelectrics and ElectricallyConductive Solids. Gordon and Breach Science Publishers, New York (1988). Ikeda T: Fundamentals of Piezoelectricity. Oxford Science Publications, New York
18. 18 Chapter 1 Introduction to Piezoelectricity(1990). Rogacheva NN: The Theory of Piezoelectric Shells and Plates. CRC Press, BocaRaton (1994). Qin QH: Fracture Mechanics of Piezoelectric Materials. WIT Press, Southampton(2001). Qin QH: Green’s Function And Boundary Elements in Multifield Materials. Elsevier,Oxford (2007). Qin QH, Yang QS: Macro-Micro Theory on Multifield Behaviour of HeterogeneousMaterials. Higher Education Press & Springer, Beijing (2008). Kistler: The Piezoelectric Effect, Theory, Design and Usage. http://www.designinfo.com/kistler/ref/tech_theory_text.htm (2010). Accessed 15 March 2011. Qin QH: Variational formulations for TFEM of piezoelectricity. International Journalof Solids and Structures 40(23), 6335-6346 (2003). Parton VZ: Fracture mechanics of piezoelectric materials. Acta Astronautica 3,671-683 (1976). Hao TH, Shen ZY: A new electric boundary condition of electric fracture mechanicsand its applications. Engineering Fracture Mechanics 47(6), 793-802 (1994). Suo Z, Kuo CM, Barnett DM, Willis JR: Fracture mechanics for piezoelectricceramics. Journal of the Mechanics and Physics of Solids 40(4), 739-765 (1992). Deeg WF: The analysis of dislocation, crack, and inclusion problems in piezoelectricsolids. PhD Thesis, Stanford University (1980). Sutradhar A, Paulino GH: The simple boundary element method for transient heatconduction in functionally graded materials. Computer Methods in Applied Mechanicsand Engineering 193(42-44), 4511-4539 (2004). Sosa H: On the fracture-mechanics of piezoelectric solids. International Journal ofSolids and Structures 29(21), 2613-2622 (1992). Zhong Z, Yu T: Electroelastic analysis of functionally graded piezoelectric materialbeams. Journal of Intelligent Material Systems and Structures 19(6), 707-713 (2008). Nelson LJ: Smart piezoelectric fibre composites. Materials Science and Technology18(11), 1245-1256 (2002). Hagood N, Bent A: Composites for structural control. US Patent, 6048622 (2000). Newnham RE, Skinner DP, Cross LE: Connectivity and piezoelectric-pyroelectriccomposites. Materials Research Bulletin 13(5), 525-536 (1978). Smith WA: The role of piezoelectric in ultrasonic transducers. IEEE 1989 UltrasonicSymposium, 755-766 (1989). Safari A, Janas V, Jadidian B: Incorporation of piezoelectric Pb(Zr,Ti)O3 fibre intoceramic/polymer composites. Proc. SPIE 2721, 240-250 (1996). Brei D, Cannon BJ: Piezoceramic hollow fiber active composites. Composites Scienceand Technology 64(2), 245-261 (2004). Chan HLW, Unsworth J: Simple model for piezoelectric ceramic polymer 1-3composites used in ultrasonic transducer applications. IEEE Transactions onUltrasonic, Ferroelectrics & Frequency Control 36, 434-441 (1989). Chan HLW, Guy IL: Piezoelectric ceramic/polymer composites for high frequencyapplications. Key Engineering Materials 92-93, 275-300 (1994). Bent AA, Hagood NW: Piezoelectric fiber composites with interdigitated electrodes.
19. References 19Journal of Intelligent Material Systems and Structures 8(11), 903-919 (1997). Bent AA, Hagood NW: Improved performance in piezoelectric fibre composites usinginterdigitated electrodes. Proc. SPIE 2441, 196-212(1995). Hagood NW, Kindel R, Ghandi K, Gaudenzi P: Improving transverse actuation ofpiezoceramics using interdigitated surface electrodes. Proc. SPIE 1917, 341-352 (1993). Cannon BJ, Brei D: Feasibility study of microfabrication by coextrusion (MFCX)hollow fibers for active composites. Journal of Intelligent Material Systems andStructures 11(9), 659-670 (2000). Fernandez JF, Dogan A, Zhang QM, Tressler JF, Newnham RE: Hollow piezoelectriccomposites. Sensors and Actuators A: Physical 51(2-3), 183-192 (1995). Williams RB, Park G, Inman DJ, Wilkie WK: An overview of composite actuatorswith piezoceramic fibers. Proc. SPIE 4753, 421-427 (2002). Zhang QM, Wang H, Cross LE: Piezoelectric tubes and tubular composites foractuator and sensor applications. Journal of Materials Science 28(14), 3962-3968(1993).